data_aluminocerite-(Ce)
_publ_requested_journal          Am.Miner.
_publ_contact_author_name        'Fabrizio Nestola'
_publ_contact_author_address 
; 
Dipartimento di Geoscienze, Università di Padova, 
Via Giotto 1, 35137, Padova,Italy
;
_publ_contact_author_email       fabrizio.nestola@unipd.it
loop_
_publ_author_name
_publ_author_address
'Nestola, Fabrizio '
;
Dipartimento di Geoscienze, Università di Padova,
 Via Giotto 1, 35137, Padova,Italy
;
'Guastoni, Alessandro'
;
Dipartimento di Geoscienze, Università di Padova,
 Via Giotto 1, 35137, Padova,Italy
;
'Camara, Fernando'
;
'C.N.R. - Istituto di Geoscienze e Georisorse - Unità di Pavia,
 Via Ferrata 1, 27100 Pavia, Italy
;
'Secco, Luciano'
;
Dipartimento di Geoscienze, Università di Padova, 
Via Giotto 1, 35137, Padova,Italy
;
'Dal Negro, Alberto'
;
Dipartimento di Geoscienze, Università di Padova,
 Via Giotto 1, 35137, Padova,Italy
;
'Pedron, D.'
;
Dipartimento di Scienze Chimiche, Università di Padova,
 Via Marzolo 1, 35131, Padova, Italy
;
'Beran, A'
;
Institute of Mineralogy and Crystallography, University of Vienna,
 Althanstrasse 14, 1090 Vienna, Austria
;


_audit_creation_method           SHELXL-97
_chemical_name_systematic        aluminocerite-(Ce)
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Al0.60 Ca0 Ce7.08 Fe0.39 O31 Si6.93'
_chemical_formula_weight         1720.86


loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ce Ce -0.2486 2.6331 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe FeP3 0.3010 0.8450 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'


_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'R 3 c'
_symmetry_int_tables_number      161


loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-y, -x, z+1/2'
'-x+y, -x, z'
'x, x-y, z+1/2'
'-x+y, y, z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-y+2/3, -x+1/3, z+5/6'
'-x+y+2/3, -x+1/3, z+1/3'
'x+2/3, x-y+1/3, z+5/6'
'-x+y+2/3, y+1/3, z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-y+1/3, -x+2/3, z+7/6'
'-x+y+1/3, -x+2/3, z+2/3'
'x+1/3, x-y+2/3, z+7/6'
'-x+y+1/3, y+2/3, z+7/6'


_cell_length_a                   10.6450(10)
_cell_length_b                   10.6450(10)
_cell_length_c                   38.019(5)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_volume                     3731.0(7)
_cell_formula_units_Z            6
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      ?
_cell_measurement_theta_max      ?


_exptl_crystal_description       ?
_exptl_crystal_colour            ?
_exptl_crystal_size_max          0.040
_exptl_crystal_size_mid          0.030
_exptl_crystal_size_min          0.025
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    4.595
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             4635
_exptl_absorpt_coefficient_mu    13.165
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?


_exptl_special_details           
;
X-red (Stoe and Cie 2001) and X-shape (Stoe and Cie 1999)
;


_diffrn_ambient_temperature      293(2)
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  ?
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            3282
_diffrn_reflns_av_R_equivalents  0.0622
_diffrn_reflns_av_sigmaI/netI    0.1241
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_k_max       17
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_limit_l_max       58
_diffrn_reflns_theta_min         3.08
_diffrn_reflns_theta_max         35.00
_reflns_number_total             1795
_reflns_number_gt                754
_reflns_threshold_expression     >2sigma(I)


_computing_data_collection       'Crysalis Red (Oxford Diffraction)'
_computing_cell_refinement       'Crysalis Red (Oxford Diffraction)'
_computing_data_reduction        'Crysalis Red (Oxford Diffraction)'
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?


_refine_special_details          
;
 Refinement of F² against ALL reflections.  The weighted R-factor wR and
 goodness of fit S are based on F², conventional R-factors R are based
 on F, with F set to zero for negative F². The threshold expression of
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is
 not relevant to the choice of reflections for refinement.  R-factors based
 on F² are statistically about twice as large as those based on F, and R-
 factors based on ALL data will be even larger.
;


_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0532P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    .
_refine_ls_extinction_method     SHELXL
_refine_ls_extinction_coef       0.000049(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.18(8)
_refine_ls_number_reflns         1795
_refine_ls_number_parameters     149
_refine_ls_number_restraints     4
_refine_ls_R_factor_all          0.1117
_refine_ls_R_factor_gt           0.0567
_refine_ls_wR_factor_ref         0.1402
_refine_ls_wR_factor_gt          0.1190
_refine_ls_goodness_of_fit_ref   0.792
_refine_ls_restrained_S_all      0.791
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000


loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Ce1 Ce 0.25920(17) 0.13369(18) 0.06808(5) 0.0233(4) Uani 0.923(10) 1 d P . .
Ce2 Ce 0.14123(18) 0.2582(2) 0.43098(7) 0.0224(4) Uani 0.820(10) 1 d P . .
Ce3 Ce 0.2572(2) 0.1337(2) 0.1759 0.0230(5) Uani 0.616(8) 1 d P . .
Si1 Si 0.3167(8) 0.1467(8) 0.36201(18) 0.0234(16) Uani 1 1 d . . .
Si2 Si 0.1499(8) 0.3268(9) 0.1372(2) 0.0231(14) Uani 1 1 d . . .
Si3 Si 0.0000 0.0000 0.2531(4) 0.027(2) Uani 1 3 d SD . .
Al1A Al 0.0000 0.0000 -0.0014(3) 0.026(2) Uani 0.61(4) 3 d SP . .
AL1B FeP3 0.0000 0.0000 -0.0014(3) 0.026(2) Uani 0.39(4) 3 d SP . .
O1 O 0.256(2) 0.090(2) 0.3228(5) 0.035(5) Uani 1 1 d . . .
O2 O 0.277(2) 0.0044(16) 0.3854(5) 0.025(4) Uani 1 1 d . . .
O3 O 0.265(3) 0.250(2) 0.3782(5) 0.034(5) Uani 1 1 d . . .
O4 O 0.083(2) 0.1684(18) 0.0297(4) 0.029(4) Uani 1 1 d . . .
O5 O 0.244(2) 0.268(2) 0.1158(5) 0.037(5) Uani 1 1 d . . .
O6 O -0.018(2) 0.269(2) 0.1227(6) 0.035(5) Uani 1 1 d . . .
O7 O 0.1637(18) 0.0719(19) 0.4679(5) 0.027(4) Uani 1 1 d . . .
O8 O 0.142(2) 0.2790(15) 0.1783(5) 0.024(3) Uani 1 1 d . . .
O9 O 0.1626(14) 0.038(2) 0.2404(5) 0.050(6) Uani 1 1 d D . .
O10 O 0.0000 0.0000 0.2972(5) 0.024(6) Uani 1 3 d SD . .
O11 O 0.0000 0.0000 0.0921(11) 0.029(7) Uani 1 3 d S . .
O12 O 0.0000 0.0000 0.1607(7) 0.018(4) Uani 1 3 d S . .
O13 O 0.0000 0.0000 0.4096(10) 0.056(12) Uani 1 3 d S . .




_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ce1 O5 2.36(2) . ?
Ce1 O8 2.452(18) 9_554 ?
Ce1 O6 2.51(2) 4 ?
Ce1 O4 2.55(2) . ?
Ce1 O11 2.558(14) . ?
Ce1 O4 2.57(2) 4 ?
Ce1 O2 2.60(2) 14_544 ?
Ce1 O3 2.74(2) 16_554 ?
Ce1 O9 2.815(19) 12_554 ?
Ce1 Si1 3.225(8) 14_544 ?
Ce1 Si1 3.307(8) 16_554 ?
Ce1 Al1A 3.562(10) . ?
Ce2 O2 2.379(18) 2 ?
Ce2 O3 2.426(19) . ?
Ce2 O9 2.463(16) 15_554 ?
Ce2 O7 2.498(19) 2 ?
Ce2 O13 2.518(13) . ?
Ce2 O7 2.536(18) . ?
Ce2 O5 2.61(2) 8 ?
Ce2 O1 2.645(19) 15_554 ?
Ce2 O6 2.80(2) 10_455 ?
Ce2 Si2 3.193(8) 8 ?
Ce2 Si2 3.227(8) 10_455 ?
Ce2 Al1A 3.506(10) 3 ?
Ce3 O8 2.41(2) . ?
Ce3 O12 2.441(6) . ?
Ce3 O6 2.47(2) 4 ?
Ce3 O2 2.517(15) 12_554 ?
Ce3 O3 2.525(18) 9_554 ?
Ce3 O8 2.55(2) 4 ?
Ce3 O9 2.655(18) . ?
Ce3 O5 2.73(2) . ?
Ce3 O1 2.970(19) 12_554 ?
Ce3 Si2 3.070(8) 4 ?
Ce3 Si2 3.168(8) . ?
Ce3 Si1 3.353(8) 12_554 ?
Si1 O3 1.58(2) . ?
Si1 O1 1.618(19) . ?
Si1 O2 1.620(18) . ?
Si1 O4 1.678(18) 8 ?
Si1 Ce1 3.225(8) 10 ?
Si1 Ce1 3.307(8) 8 ?
Si1 Ce3 3.353(8) 18_544 ?
Si2 O7 1.628(18) 16_554 ?
Si2 O8 1.63(2) . ?
Si2 O5 1.64(2) . ?
Si2 O6 1.67(2) . ?
Si2 Ce3 3.070(8) 2 ?
Si2 Ce2 3.193(8) 16_554 ?
Si2 Ce2 3.227(8) 14_554 ?
Si3 O10 1.676(18) . ?
Si3 O9 1.640(11) 4 ?
Si3 O9 1.640(11) . ?
Si3 O9 1.640(11) 2 ?
Al1A O7 1.911(19) 3_554 ?
Al1A O7 1.911(19) 5_554 ?
Al1A O7 1.911(19) 6_554 ?
Al1A O4 1.951(19) . ?
Al1A O4 1.951(19) 4 ?
Al1A O4 1.951(19) 2 ?
Al1A Ce2 3.506(10) 3_554 ?
Al1A Ce2 3.506(10) 5_554 ?
Al1A Ce2 3.506(10) 6_554 ?
Al1A Ce1 3.562(10) 2 ?
Al1A Ce1 3.562(10) 4 ?
O1 Ce2 2.645(19) 9_554 ?
O1 Ce3 2.970(19) 18_544 ?
O2 Ce2 2.379(18) 4 ?
O2 Ce3 2.517(15) 18_544 ?
O2 Ce1 2.60(2) 10 ?
O3 Ce3 2.525(18) 15_554 ?
O3 Ce1 2.74(2) 8 ?
O4 Si1 1.678(18) 16_554 ?
O4 Ce1 2.57(2) 2 ?
O5 Ce2 2.61(2) 16_554 ?
O6 Ce3 2.47(2) 2 ?
O6 Ce1 2.51(2) 2 ?
O6 Ce2 2.80(2) 14_554 ?
O7 Si2 1.628(18) 8 ?
O7 AL1B 1.911(19) 3 ?
O7 Al1A 1.911(19) 3 ?
O7 Ce2 2.498(19) 4 ?
O8 Ce1 2.452(18) 15_554 ?
O8 Ce3 2.55(2) 2 ?
O9 Ce2 2.463(16) 9_554 ?
O9 Ce1 2.815(19) 18_544 ?
O11 Ce1 2.558(14) 4 ?
O11 Ce1 2.558(14) 2 ?
O12 Ce3 2.441(6) 4 ?
O12 Ce3 2.441(6) 2 ?
O13 Ce2 2.518(13) 2 ?
O13 Ce2 2.518(13) 4 ?


loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O5 Ce1 O8 135.8(7) . 9_554 ?
O5 Ce1 O6 73.8(7) . 4 ?
O8 Ce1 O6 131.4(7) 9_554 4 ?
O5 Ce1 O4 94.4(6) . . ?
O8 Ce1 O4 79.7(6) 9_554 . ?
O6 Ce1 O4 145.4(6) 4 . ?
O5 Ce1 O11 71.5(8) . . ?
O8 Ce1 O11 139.7(9) 9_554 . ?
O6 Ce1 O11 77.9(8) 4 . ?
O4 Ce1 O11 67.5(8) . . ?
O5 Ce1 O4 138.0(6) . 4 ?
O8 Ce1 O4 77.8(6) 9_554 4 ?
O6 Ce1 O4 103.8(7) 4 4 ?
O4 Ce1 O4 63.4(7) . 4 ?
O11 Ce1 O4 67.1(8) . 4 ?
O5 Ce1 O2 142.5(6) . 14_544 ?
O8 Ce1 O2 69.5(7) 9_554 14_544 ?
O6 Ce1 O2 69.6(6) 4 14_544 ?
O4 Ce1 O2 120.4(6) . 14_544 ?
O11 Ce1 O2 107.4(4) . 14_544 ?
O4 Ce1 O2 61.0(5) 4 14_544 ?
O5 Ce1 O3 70.7(6) . 16_554 ?
O8 Ce1 O3 69.3(7) 9_554 16_554 ?
O6 Ce1 O3 139.1(7) 4 16_554 ?
O4 Ce1 O3 57.8(5) . 16_554 ?
O11 Ce1 O3 108.5(4) . 16_554 ?
O4 Ce1 O3 116.0(6) 4 16_554 ?
O2 Ce1 O3 138.2(5) 14_544 16_554 ?
O5 Ce1 O9 76.2(6) . 12_554 ?
O8 Ce1 O9 68.2(5) 9_554 12_554 ?
O6 Ce1 O9 92.4(6) 4 12_554 ?
O4 Ce1 O9 116.7(5) . 12_554 ?
O11 Ce1 O9 147.7(7) . 12_554 ?
O4 Ce1 O9 144.9(5) 4 12_554 ?
O2 Ce1 O9 97.5(4) 14_544 12_554 ?
O3 Ce1 O9 60.1(5) 16_554 12_554 ?
O5 Ce1 Si1 153.4(5) . 14_544 ?
O8 Ce1 Si1 70.8(5) 9_554 14_544 ?
O6 Ce1 Si1 86.1(5) 4 14_544 ?
O4 Ce1 Si1 92.5(4) . 14_544 ?
O11 Ce1 Si1 87.5(5) . 14_544 ?
O4 Ce1 Si1 31.1(4) 4 14_544 ?
O2 Ce1 Si1 29.9(4) 14_544 14_544 ?
O3 Ce1 Si1 133.5(4) 16_554 14_544 ?
O9 Ce1 Si1 122.8(4) 12_554 14_544 ?
O5 Ce1 Si1 77.9(5) . 16_554 ?
O8 Ce1 Si1 75.8(6) 9_554 16_554 ?
O6 Ce1 Si1 150.6(5) 4 16_554 ?
O4 Ce1 Si1 29.9(4) . 16_554 ?
O11 Ce1 Si1 85.8(5) . 16_554 ?
O4 Ce1 Si1 91.9(4) 4 16_554 ?
O2 Ce1 Si1 139.4(4) 14_544 16_554 ?
O3 Ce1 Si1 28.4(4) 16_554 16_554 ?
O9 Ce1 Si1 88.4(3) 12_554 16_554 ?
Si1 Ce1 Si1 117.8(2) 14_544 16_554 ?
O5 Ce1 Al1A 122.6(5) . . ?
O8 Ce1 Al1A 71.0(4) 9_554 . ?
O6 Ce1 Al1A 132.5(5) 4 . ?
O4 Ce1 Al1A 32.1(4) . . ?
O11 Ce1 Al1A 68.7(8) . . ?
O4 Ce1 Al1A 32.2(4) 4 . ?
O2 Ce1 Al1A 88.9(4) 14_544 . ?
O3 Ce1 Al1A 84.6(4) 16_554 . ?
O9 Ce1 Al1A 133.2(4) 12_554 . ?
Si1 Ce1 Al1A 60.38(14) 14_544 . ?
Si1 Ce1 Al1A 59.69(13) 16_554 . ?
O2 Ce2 O3 77.4(6) 2 . ?
O2 Ce2 O9 76.8(6) 2 15_554 ?
O3 Ce2 O9 69.5(6) . 15_554 ?
O2 Ce2 O7 93.7(5) 2 2 ?
O3 Ce2 O7 139.1(7) . 2 ?
O9 Ce2 O7 147.8(6) 15_554 2 ?
O2 Ce2 O13 77.4(7) 2 . ?
O3 Ce2 O13 74.5(9) . . ?
O9 Ce2 O13 139.3(9) 15_554 . ?
O7 Ce2 O13 64.7(8) 2 . ?
O2 Ce2 O7 140.5(6) 2 . ?
O3 Ce2 O7 99.5(6) . . ?
O9 Ce2 O7 139.7(6) 15_554 . ?
O7 Ce2 O7 62.7(7) 2 . ?
O13 Ce2 O7 64.1(8) . . ?
O2 Ce2 O5 146.0(6) 2 8 ?
O3 Ce2 O5 72.2(7) . 8 ?
O9 Ce2 O5 78.6(6) 15_554 8 ?
O7 Ce2 O5 119.2(6) 2 8 ?
O13 Ce2 O5 107.9(5) . 8 ?
O7 Ce2 O5 61.2(6) . 8 ?
O2 Ce2 O1 130.7(6) 2 15_554 ?
O3 Ce2 O1 130.9(7) . 15_554 ?
O9 Ce2 O1 78.8(6) 15_554 15_554 ?
O7 Ce2 O1 84.9(6) 2 15_554 ?
O13 Ce2 O1 141.2(9) . 15_554 ?
O7 Ce2 O1 81.1(6) . 15_554 ?
O5 Ce2 O1 65.4(6) 8 15_554 ?
O2 Ce2 O6 67.9(6) 2 10_455 ?
O3 Ce2 O6 142.1(6) . 10_455 ?
O9 Ce2 O6 87.8(6) 15_554 10_455 ?
O7 Ce2 O6 60.3(6) 2 10_455 ?
O13 Ce2 O6 110.7(5) . 10_455 ?
O7 Ce2 O6 116.8(6) . 10_455 ?
O5 Ce2 O6 134.1(7) 8 10_455 ?
O1 Ce2 O6 69.1(6) 15_554 10_455 ?
O2 Ce2 Si2 158.0(5) 2 8 ?
O3 Ce2 Si2 85.1(5) . 8 ?
O9 Ce2 Si2 109.5(5) 15_554 8 ?
O7 Ce2 Si2 90.9(4) 2 8 ?
O13 Ce2 Si2 85.2(5) . 8 ?
O7 Ce2 Si2 30.4(4) . 8 ?
O5 Ce2 Si2 30.9(5) 8 8 ?
O1 Ce2 Si2 71.1(4) 15_554 8 ?
O6 Ce2 Si2 132.1(5) 10_455 8 ?
O2 Ce2 Si2 76.4(4) 2 10_455 ?
O3 Ce2 Si2 149.3(6) . 10_455 ?
O9 Ce2 Si2 118.8(4) 15_554 10_455 ?
O7 Ce2 Si2 29.7(4) 2 10_455 ?
O13 Ce2 Si2 84.5(5) . 10_455 ?
O7 Ce2 Si2 90.8(4) . 10_455 ?
O5 Ce2 Si2 136.8(5) 8 10_455 ?
O1 Ce2 Si2 79.1(5) 15_554 10_455 ?
O6 Ce2 Si2 31.1(4) 10_455 10_455 ?
Si2 Ce2 Si2 115.6(3) 8 10_455 ?
O2 Ce2 Al1A 123.1(4) 2 3 ?
O3 Ce2 Al1A 127.3(5) . 3 ?
O9 Ce2 Al1A 154.1(4) 15_554 3 ?
O7 Ce2 Al1A 31.8(4) 2 3 ?
O13 Ce2 Al1A 66.0(8) . 3 ?
O7 Ce2 Al1A 32.0(4) . 3 ?
O5 Ce2 Al1A 88.0(5) 8 3 ?
O1 Ce2 Al1A 75.5(4) 15_554 3 ?
O6 Ce2 Al1A 85.7(4) 10_455 3 ?
Si2 Ce2 Al1A 59.07(16) 8 3 ?
Si2 Ce2 Al1A 58.79(16) 10_455 3 ?
O8 Ce3 O12 66.4(4) . . ?
O8 Ce3 O6 125.8(7) . 4 ?
O12 Ce3 O6 84.4(7) . 4 ?
O8 Ce3 O2 71.5(6) . 12_554 ?
O12 Ce3 O2 130.8(6) . 12_554 ?
O6 Ce3 O2 142.9(7) 4 12_554 ?
O8 Ce3 O3 141.6(6) . 9_554 ?
O12 Ce3 O3 132.7(6) . 9_554 ?
O6 Ce3 O3 91.8(6) 4 9_554 ?
O2 Ce3 O3 73.1(6) 12_554 9_554 ?
O8 Ce3 O8 127.9(5) . 4 ?
O12 Ce3 O8 64.4(4) . 4 ?
O6 Ce3 O8 64.6(6) 4 4 ?
O2 Ce3 O8 135.2(6) 12_554 4 ?
O3 Ce3 O8 71.5(7) 9_554 4 ?
O8 Ce3 O9 89.5(6) . . ?
O12 Ce3 O9 84.0(7) . . ?
O6 Ce3 O9 133.3(7) 4 . ?
O2 Ce3 O9 71.1(6) 12_554 . ?
O3 Ce3 O9 65.0(6) 9_554 . ?
O8 Ce3 O9 69.6(6) 4 . ?
O8 Ce3 O5 61.5(6) . . ?
O12 Ce3 O5 76.9(7) . . ?
O6 Ce3 O5 68.2(6) 4 . ?
O2 Ce3 O5 104.4(6) 12_554 . ?
O3 Ce3 O5 143.9(7) 9_554 . ?
O8 Ce3 O5 120.3(6) 4 . ?
O9 Ce3 O5 149.8(5) . . ?
O8 Ce3 O1 78.8(5) . 12_554 ?
O12 Ce3 O1 133.6(5) . 12_554 ?
O6 Ce3 O1 92.7(6) 4 12_554 ?
O2 Ce3 O1 55.8(5) 12_554 12_554 ?
O3 Ce3 O1 93.5(7) 9_554 12_554 ?
O8 Ce3 O1 151.6(6) 4 12_554 ?
O9 Ce3 O1 126.7(5) . 12_554 ?
O5 Ce3 O1 59.5(6) . 12_554 ?
O8 Ce3 Si2 131.9(5) . 4 ?
O12 Ce3 Si2 68.5(3) . 4 ?
O6 Ce3 Si2 32.8(5) 4 4 ?
O2 Ce3 Si2 156.2(5) 12_554 4 ?
O3 Ce3 Si2 83.2(5) 9_554 4 ?
O8 Ce3 Si2 32.1(4) 4 4 ?
O9 Ce3 Si2 101.6(5) . 4 ?
O5 Ce3 Si2 92.9(5) . 4 ?
O1 Ce3 Si2 124.7(4) 12_554 4 ?
O8 Ce3 Si2 30.3(5) . . ?
O12 Ce3 Si2 66.8(3) . . ?
O6 Ce3 Si2 97.0(5) 4 . ?
O2 Ce3 Si2 89.0(5) 12_554 . ?
O3 Ce3 Si2 159.6(6) 9_554 . ?
O8 Ce3 Si2 128.9(5) 4 . ?
O9 Ce3 Si2 119.1(4) . . ?
O5 Ce3 Si2 31.2(4) . . ?
O1 Ce3 Si2 67.7(4) 12_554 . ?
Si2 Ce3 Si2 113.7(3) 4 . ?
O8 Ce3 Si1 68.8(4) . 12_554 ?
O12 Ce3 Si1 135.05(16) . 12_554 ?
O6 Ce3 Si1 120.9(5) 4 12_554 ?
O2 Ce3 Si1 27.6(4) 12_554 12_554 ?
O3 Ce3 Si1 86.4(6) 9_554 12_554 ?
O8 Ce3 Si1 157.7(5) 4 12_554 ?
O9 Ce3 Si1 98.6(4) . 12_554 ?
O5 Ce3 Si1 79.6(4) . 12_554 ?
O1 Ce3 Si1 28.8(4) 12_554 12_554 ?
Si2 Ce3 Si1 150.7(2) 4 12_554 ?
Si2 Ce3 Si1 73.25(16) . 12_554 ?
O3 Si1 O1 113.7(11) . . ?
O3 Si1 O2 114.7(10) . . ?
O1 Si1 O2 106.9(10) . . ?
O3 Si1 O4 103.7(12) . 8 ?
O1 Si1 O4 112.3(10) . 8 ?
O2 Si1 O4 105.4(11) . 8 ?
O3 Si1 Ce1 123.0(8) . 10 ?
O1 Si1 Ce1 123.2(8) . 10 ?
O2 Si1 Ce1 53.1(7) . 10 ?
O4 Si1 Ce1 52.3(7) 8 10 ?
O3 Si1 Ce1 55.6(9) . 8 ?
O1 Si1 Ce1 137.7(8) . 8 ?
O2 Si1 Ce1 114.6(7) . 8 ?
O4 Si1 Ce1 49.1(8) 8 8 ?
Ce1 Si1 Ce1 78.64(17) 10 8 ?
O3 Si1 Ce3 143.7(9) . 18_544 ?
O1 Si1 Ce3 62.3(7) . 18_544 ?
O2 Si1 Ce3 46.1(6) . 18_544 ?
O4 Si1 Ce3 111.0(8) 8 18_544 ?
Ce1 Si1 Ce3 73.97(17) 10 18_544 ?
Ce1 Si1 Ce3 152.6(3) 8 18_544 ?
O7 Si2 O8 109.0(10) 16_554 . ?
O7 Si2 O5 106.3(10) 16_554 . ?
O8 Si2 O5 107.6(11) . . ?
O7 Si2 O6 108.6(10) 16_554 . ?
O8 Si2 O6 108.7(12) . . ?
O5 Si2 O6 116.4(12) . . ?
O7 Si2 Ce3 130.8(7) 16_554 2 ?
O8 Si2 Ce3 56.0(7) . 2 ?
O5 Si2 Ce3 122.8(8) . 2 ?
O6 Si2 Ce3 53.4(8) . 2 ?
O7 Si2 Ce3 125.0(7) 16_554 . ?
O8 Si2 Ce3 48.3(8) . . ?
O5 Si2 Ce3 59.6(7) . . ?
O6 Si2 Ce3 125.6(8) . . ?
Ce3 Si2 Ce3 82.4(2) 2 . ?
O7 Si2 Ce2 51.9(7) 16_554 16_554 ?
O8 Si2 Ce2 122.5(8) . 16_554 ?
O5 Si2 Ce2 54.4(7) . 16_554 ?
O6 Si2 Ce2 128.5(8) . 16_554 ?
Ce3 Si2 Ce2 176.9(3) 2 16_554 ?
Ce3 Si2 Ce2 94.69(19) . 16_554 ?
O7 Si2 Ce2 49.5(7) 16_554 14_554 ?
O8 Si2 Ce2 132.8(8) . 14_554 ?
O5 Si2 Ce2 118.3(8) . 14_554 ?
O6 Si2 Ce2 60.2(7) . 14_554 ?
Ce3 Si2 Ce2 102.9(2) 2 14_554 ?
Ce3 Si2 Ce2 174.1(3) . 14_554 ?
Ce2 Si2 Ce2 80.0(2) 16_554 14_554 ?
O10 Si3 O9 107.1(8) . 4 ?
O10 Si3 O9 107.1(8) . . ?
O9 Si3 O9 111.7(8) 4 . ?
O10 Si3 O9 107.1(8) . 2 ?
O9 Si3 O9 111.7(8) 4 2 ?
O9 Si3 O9 111.7(8) . 2 ?
O7 Al1A O7 86.6(10) 3_554 5_554 ?
O7 Al1A O7 86.6(10) 3_554 6_554 ?
O7 Al1A O7 86.6(10) 5_554 6_554 ?
O7 Al1A O4 177.2(11) 3_554 . ?
O7 Al1A O4 91.3(8) 5_554 . ?
O7 Al1A O4 95.1(8) 6_554 . ?
O7 Al1A O4 91.3(8) 3_554 4 ?
O7 Al1A O4 95.1(8) 5_554 4 ?
O7 Al1A O4 177.2(11) 6_554 4 ?
O4 Al1A O4 87.1(8) . 4 ?
O7 Al1A O4 95.1(8) 3_554 2 ?
O7 Al1A O4 177.2(11) 5_554 2 ?
O7 Al1A O4 91.3(8) 6_554 2 ?
O4 Al1A O4 87.1(8) . 2 ?
O4 Al1A O4 87.1(8) 4 2 ?
O7 Al1A Ce2 44.8(6) 3_554 3_554 ?
O7 Al1A Ce2 95.2(8) 5_554 3_554 ?
O7 Al1A Ce2 43.6(6) 6_554 3_554 ?
O4 Al1A Ce2 137.3(6) . 3_554 ?
O4 Al1A Ce2 133.9(7) 4 3_554 ?
O4 Al1A Ce2 84.5(5) 2 3_554 ?
O7 Al1A Ce2 43.6(6) 3_554 5_554 ?
O7 Al1A Ce2 44.8(6) 5_554 5_554 ?
O7 Al1A Ce2 95.2(8) 6_554 5_554 ?
O4 Al1A Ce2 133.9(7) . 5_554 ?
O4 Al1A Ce2 84.5(5) 4 5_554 ?
O4 Al1A Ce2 137.3(6) 2 5_554 ?
Ce2 Al1A Ce2 72.1(2) 3_554 5_554 ?
O7 Al1A Ce2 95.2(8) 3_554 6_554 ?
O7 Al1A Ce2 43.6(6) 5_554 6_554 ?
O7 Al1A Ce2 44.8(6) 6_554 6_554 ?
O4 Al1A Ce2 84.5(5) . 6_554 ?
O4 Al1A Ce2 137.3(6) 4 6_554 ?
O4 Al1A Ce2 133.9(7) 2 6_554 ?
Ce2 Al1A Ce2 72.1(2) 3_554 6_554 ?
Ce2 Al1A Ce2 72.1(2) 5_554 6_554 ?
O7 Al1A Ce1 134.0(5) 3_554 . ?
O7 Al1A Ce1 85.6(6) 5_554 . ?
O7 Al1A Ce1 137.9(6) 6_554 . ?
O4 Al1A Ce1 43.9(6) . . ?
O4 Al1A Ce1 44.6(7) 4 . ?
O4 Al1A Ce1 94.9(7) 2 . ?
Ce2 Al1A Ce1 178.44(15) 3_554 . ?
Ce2 Al1A Ce1 107.55(4) 5_554 . ?
Ce2 Al1A Ce1 109.27(4) 6_554 . ?
O7 Al1A Ce1 137.9(6) 3_554 2 ?
O7 Al1A Ce1 134.0(5) 5_554 2 ?
O7 Al1A Ce1 85.6(6) 6_554 2 ?
O4 Al1A Ce1 44.6(7) . 2 ?
O4 Al1A Ce1 94.9(7) 4 2 ?
O4 Al1A Ce1 43.9(6) 2 2 ?
Ce2 Al1A Ce1 109.27(4) 3_554 2 ?
Ce2 Al1A Ce1 178.44(15) 5_554 2 ?
Ce2 Al1A Ce1 107.55(4) 6_554 2 ?
Ce1 Al1A Ce1 71.0(2) . 2 ?
O7 Al1A Ce1 85.6(6) 3_554 4 ?
O7 Al1A Ce1 137.9(6) 5_554 4 ?
O7 Al1A Ce1 134.0(5) 6_554 4 ?
O4 Al1A Ce1 94.9(7) . 4 ?
O4 Al1A Ce1 43.9(6) 4 4 ?
O4 Al1A Ce1 44.6(7) 2 4 ?
Ce2 Al1A Ce1 107.55(4) 3_554 4 ?
Ce2 Al1A Ce1 109.27(4) 5_554 4 ?
Ce2 Al1A Ce1 178.44(15) 6_554 4 ?
Ce1 Al1A Ce1 71.0(2) . 4 ?
Ce1 Al1A Ce1 71.0(2) 2 4 ?
Si1 O1 Ce2 124.9(10) . 9_554 ?
Si1 O1 Ce3 88.8(8) . 18_544 ?
Ce2 O1 Ce3 112.7(7) 9_554 18_544 ?
Si1 O2 Ce2 141.0(11) . 4 ?
Si1 O2 Ce3 106.3(9) . 18_544 ?
Ce2 O2 Ce3 96.2(6) 4 18_544 ?
Si1 O2 Ce1 97.0(9) . 10 ?
Ce2 O2 Ce1 109.6(7) 4 10 ?
Ce3 O2 Ce1 101.4(6) 18_544 10 ?
Si1 O3 Ce2 137.0(11) . . ?
Si1 O3 Ce3 124.6(10) . 15_554 ?
Ce2 O3 Ce3 94.8(7) . 15_554 ?
Si1 O3 Ce1 96.0(10) . 8 ?
Ce2 O3 Ce1 93.9(7) . 8 ?
Ce3 O3 Ce1 98.8(7) 15_554 8 ?
Si1 O4 Al1A 141.3(11) 16_554 . ?
Si1 O4 Ce1 101.0(10) 16_554 . ?
Al1A O4 Ce1 104.0(8) . . ?
Si1 O4 Ce1 96.5(9) 16_554 2 ?
Al1A O4 Ce1 103.2(9) . 2 ?
Ce1 O4 Ce1 108.0(6) . 2 ?
Si2 O5 Ce1 148.1(12) . . ?
Si2 O5 Ce2 94.7(9) . 16_554 ?
Ce1 O5 Ce2 99.1(7) . 16_554 ?
Si2 O5 Ce3 89.2(9) . . ?
Ce1 O5 Ce3 106.9(7) . . ?
Ce2 O5 Ce3 122.4(8) 16_554 . ?
Si2 O6 Ce3 93.9(9) . 2 ?
Si2 O6 Ce1 127.5(11) . 2 ?
Ce3 O6 Ce1 110.9(8) 2 2 ?
Si2 O6 Ce2 88.7(8) . 14_554 ?
Ce3 O6 Ce2 138.3(8) 2 14_554 ?
Ce1 O6 Ce2 99.9(7) 2 14_554 ?
Si2 O7 AL1B 138.8(13) 8 3 ?
Si2 O7 Al1A 138.8(13) 8 3 ?
AL1B O7 Al1A 0.0(6) 3 3 ?
Si2 O7 Ce2 100.8(8) 8 4 ?
AL1B O7 Ce2 104.6(7) 3 4 ?
Al1A O7 Ce2 104.6(7) 3 4 ?
Si2 O7 Ce2 97.7(8) 8 . ?
AL1B O7 Ce2 103.2(7) 3 . ?
Al1A O7 Ce2 103.2(7) 3 . ?
Ce2 O7 Ce2 110.2(7) 4 . ?
Si2 O8 Ce3 101.4(10) . . ?
Si2 O8 Ce1 134.8(9) . 15_554 ?
Ce3 O8 Ce1 108.9(8) . 15_554 ?
Si2 O8 Ce3 91.9(9) . 2 ?
Ce3 O8 Ce3 111.9(5) . 2 ?
Ce1 O8 Ce3 106.4(8) 15_554 2 ?
Si3 O9 Ce2 134.1(11) . 9_554 ?
Si3 O9 Ce3 121.3(11) . . ?
Ce2 O9 Ce3 90.8(4) 9_554 . ?
Si3 O9 Ce1 115.6(9) . 18_544 ?
Ce2 O9 Ce1 91.3(5) 9_554 18_544 ?
Ce3 O9 Ce1 94.0(5) . 18_544 ?
Ce1 O11 Ce1 108.0(9) 4 . ?
Ce1 O11 Ce1 108.0(9) 4 2 ?
Ce1 O11 Ce1 108.0(9) . 2 ?
Ce3 O12 Ce3 114.6(5) . 4 ?
Ce3 O12 Ce3 114.6(5) . 2 ?
Ce3 O12 Ce3 114.6(5) 4 2 ?
Ce2 O13 Ce2 110.1(8) . 2 ?
Ce2 O13 Ce2 110.1(8) . 4 ?
Ce2 O13 Ce2 110.1(8) 2 4 ?


_diffrn_measured_fraction_theta_max 0.963
_diffrn_reflns_theta_full        35.00
_diffrn_measured_fraction_theta_full 0.963
_refine_diff_density_max         4.988
_refine_diff_density_min         -2.406
_refine_diff_density_rms         0.421